Syntheses, Structures, Optical and Magnetic Properties of Ba2MLnSe5 (M = Ga, In; Ln= Y, Nd, Sm, Gd, Dy, Er)
Wenlong Yin; Kai Feng; Wendong Wang; Youguo Shi; Wenyu Hao; Jiyong Yao; Yicheng Wu; Inorganic Chemistry 51 (2012) 6860–6867; doi:10.1021/ic300604a

data_4329516
_publ_section_title
;
 Syntheses, Structures, Optical and Magnetic Properties of Ba2MLnSe5 (M =
 Ga, In; Ln= Y, Nd, Sm, Gd, Dy, Er)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6860
_journal_page_last               6867
_journal_paper_doi               10.1021/ic300604a
_journal_volume                  51
_journal_year                    2012
_chemical_formula_sum            'Ba2 Dy Ga Se5'
_chemical_formula_weight         901.70
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2012-03-19 # Formatted by publCIF
;
_cell_angle_alpha                103.53(3)
_cell_angle_beta                 103.07(3)
_cell_angle_gamma                107.43(3)
_cell_formula_units_Z            2
_cell_length_a                   7.2772(15)
_cell_length_b                   8.6543(17)
_cell_length_c                   9.3792(19)
_cell_measurement_reflns_used    2174
_cell_measurement_temperature    153(2)
_cell_measurement_theta_max      30.9950
_cell_measurement_theta_min      2.3569
_cell_volume                     519.2(3)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  Diamond
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      153(2)
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.973
_diffrn_measured_fraction_theta_max 0.973
_diffrn_measurement_device_type  'Rigaku AFC10 diffractometer'
_diffrn_measurement_method       dtprofit.ref
_diffrn_radiation_monochromator  'Graphite Monochromator'
_diffrn_radiation_source         'Rotating Anode'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0586
_diffrn_reflns_av_sigmaI/netI    0.0908
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            6669
_diffrn_reflns_theta_full        31.00
_diffrn_reflns_theta_max         31.00
_diffrn_reflns_theta_min         2.89
_exptl_absorpt_coefficient_mu    34.607
_exptl_absorpt_correction_T_max  0.068
_exptl_absorpt_correction_T_min  0.011
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    5.767
_exptl_crystal_description       chunk
_exptl_crystal_F_000             758
_exptl_crystal_size_max          0.1820
_exptl_crystal_size_mid          0.1200
_exptl_crystal_size_min          0.0770
_refine_diff_density_max         3.234
_refine_diff_density_min         -3.982
_refine_diff_density_rms         0.597
_refine_ls_extinction_coef       0.00211(17)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.870
_refine_ls_matrix_type           full
_refine_ls_number_parameters     83
_refine_ls_number_reflns         3233
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.870
_refine_ls_R_factor_all          0.0562
_refine_ls_R_factor_gt           0.0418
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0400P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0935
_refine_ls_wR_factor_ref         0.0999
_reflns_number_gt                2522
_reflns_number_total             3233
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic300604a_si_001_05.cif
_cod_data_source_block           Ba2GaDySe5
_cod_original_cell_volume        519.26(26)
_cod_database_code               4329516